Crystal growth of metal tellurides from a boron-tellurium mixture: MTr<sub>2</sub>Te<sub>4</sub> (M = Sr, Eu; Tr = In, Ga).
Jana, Subhendu; Chirantha Edirisinghe, E. A.; Mongkhonratanachai, Machima; Maggard, Paul A.; Dalton transactions (Cambridge, England : 2003) 55 (2026) 4574–4583; doi:10.1039/d6dt00156d

data_7720281
_publ_section_title
;
 Crystal growth of metal tellurides from a boron-tellurium mixture:
 MTr<sub>2</sub>Te<sub>4</sub> (M = Sr, Eu; Tr = In, Ga).
;
_journal_issue                   11
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              4574
_journal_page_last               4583
_journal_paper_doi               10.1039/d6dt00156d
_journal_volume                  55
_journal_year                    2026
_chemical_formula_moiety         'Eu Ga2 Te4'
_chemical_formula_sum            'Eu Ga2 Te4'
_chemical_formula_weight         801.80
_space_group_crystal_system      orthorhombic
_space_group_IT_number           74
_space_group_name_Hall           '-I 2b 2'
_space_group_name_H-M_alt        'I m m a'
_audit_creation_date             2025-01-08
_audit_creation_method
;
Olex2 1.5
(compiled 2024.02.16 svn.r378c4104 for OlexSys, GUI svn.r6928)
;
_audit_update_record
;
2025-01-08 deposited with the CCDC.	2026-02-23 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.5596(5)
_cell_length_b                   23.0747(9)
_cell_length_c                   6.7187(3)
_cell_measurement_reflns_used    3939
_cell_measurement_temperature    300
_cell_measurement_theta_max      30.53
_cell_measurement_theta_min      3.53
_cell_volume                     1792.11(13)
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2019/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      300.00
_diffrn_measured_fraction_theta_full 0.971
_diffrn_measured_fraction_theta_max 0.979
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0336
_diffrn_reflns_av_unetI/netI     0.0184
_diffrn_reflns_Laue_measured_fraction_full 0.971
_diffrn_reflns_Laue_measured_fraction_max 0.979
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       30
_diffrn_reflns_limit_k_min       -29
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            11320
_diffrn_reflns_point_group_measured_fraction_full 0.971
_diffrn_reflns_point_group_measured_fraction_max 0.979
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.280
_diffrn_reflns_theta_min         3.507
_exptl_absorpt_coefficient_mu    25.552
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   multi-scan
_exptl_crystal_colour            Black
_exptl_crystal_density_diffrn    5.943
_exptl_crystal_description       block
_exptl_crystal_F_000             2664
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.02
_exptl_transmission_factor_max   0.7461
_exptl_transmission_factor_min   0.4608
_refine_diff_density_max         3.341
_refine_diff_density_min         -0.865
_refine_diff_density_rms         0.199
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.080
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     43
_refine_ls_number_reflns         1169
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.080
_refine_ls_R_factor_all          0.0270
_refine_ls_R_factor_gt           0.0212
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0351P)^2^+1.2444P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0591
_refine_ls_wR_factor_ref         0.0639
_reflns_Friedel_coverage         0.000
_reflns_number_gt                883
_reflns_number_total             1169
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d6dt00156d2.cif
_cod_data_source_block           euga2te4
_cod_depositor_comments
'Adding full bibliography for 7720281--7720283.cif.'
_cod_database_code               7720281
_shelx_shelxl_version_number     2019/3
_exptl_absorpt_special_details   SADABS
_olex2_refinement_description
;
;
_shelx_res_checksum              40962
_olex2_submission_special_instructions 'No special instructions were received'